General rights Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
Users may download and print one copy of any publication from the public portal for the purpose of private study or research.
You may not further distribute the material or use it for any profit-making activity or commercial gain
You may freely distribute the URL identifying the publication in the public portal If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately and investigate your claim.
Downloaded from orbit.dtu.dk on: Sep 01, 2021
Strategies of Coping with Deactivation of NH3-SCR Catalysts Due to Biomass Firing
Schill, Leonhard; Fehrmann, Rasmus
Publication date: 2018
Document Version Publisher's PDF, also known as Version of record
Link back to DTU Orbit
Citation (APA): Schill, L., & Fehrmann, R. (2018). Strategies of Coping with Deactivation of NH3-SCR Catalysts Due to Biomass Firing. Catalysts, 8(4), . https://doi.org/10.3390/catal8040135
Leonhard Schill and Rasmus Fehrmann *
Center for Catalysis and Sustainable Chemistry, Department of Chemistry, Building 207, Technical University of Denmark, DK-2800 Kongens Lyngby, Denmark; [email protected]
* Correspondence: [email protected]
; Tel.: +45-25-23-89
Received: 28 February 2018; Accepted: 22 March 2018; Published: 30 March 2018
Abstract: Firing of biomass can lead to rapid deactivation of the vanadia-based NH3-SCR catalyst, which reduces NOx to harmless N2. The deactivation is mostly due to the high potassium content in biomasses, which results in submicron aerosols containing mostly KCl and K2SO4. The main mode of deactivation is neutralization of the catalyst’s acid sites. Four ways of dealing with high potassium contents were identified: (1) potassium removal by adsorption, (2) tail-end placement of the SCR unit, (3) coating SCR monoliths with a protective layer, and (4) intrinsically potassium tolerant catalysts. Addition of alumino silicates, often in the form of coal fly ash, is an industrially proven method of removing K aerosols from flue gases. Tail-end placement of the SCR unit was also reported to result in acceptable catalyst stability; however, flue-gas reheating after the flue gas desulfurization is, at present, unavoidable due to the lack of sulfur and water tolerant low temperature catalysts. Coating the shaped catalysts with thin layers of, e.g., MgO or sepiolite reduces the K uptake by hindering the diffusion of K+ into the catalyst pore system. Intrinsically potassium tolerant catalysts typically contain a high number of acid sites. This can be achieved by, e.g., using zeolites as support, replacing WO3 with heteropoly acids, and by preparing highly loaded, high surface area, very active V2O5/TiO2 catalyst using a special sol-gel method.
Keywords: biomass firing; NH3 SCR; potassium resistant catalysts; alumino silicate addition; coal ash; tail end placement; basic coating; KCl; aerosol
The amount of electricity generated from firing solid biomass has been rising steeply in Europe over the last decades and is expected to continue to do so . Similar trends are seen in other regions of the world [2,3]. Replacing fossil fuels, especially coal, by biomass aims at reducing the CO2 emissions associated with thermal power plants [2,4–7]. Even though renewable energy sources like solar and wind power are more and more cost competitive  and make up an increasing share of power generation in most regions , some thermal power plant capacity is still needed due to the renewables’ fluctuating nature and the current lack of sufficient storage capacity . Firing and co-firing of biomass can cause several problems in the power plant like slagging and fouling problems in boilers , ash deposition on heat exchangers, and increased catalyst deactivation in the NOx
removing unit [12–18]. This review deals with the last-mentioned problem. NOx gases cause formation of photochemical smog, acid rain (HNO3), and ground level ozone
formation. These conditions in turn have adverse consequences on human life and ecosystems. NOx emissions from power plants can be reduced by modifications to the combustion process (primary measures) or post-combustion techniques (secondary measures). Secondary measures are typically more expensive but also afford a higher degree of NOx removal. Due to ever stricter environmental regulations, secondary measures are increasingly needed for power plants to be compliant. The highest
Catalysts 2018, 8, 135; doi:10.3390/catal8040135 www.mdpi.com/journal/catalysts
Catalysts 2018, 8, 135 2 of 11
degree of NOx removal is achieved with selective catalytic reduction (SCR) using ammonia as the reductant [18,19]. The most widespread kind of catalyst is V2O5-WO3/TiO2 (VWT) [20,21]. The loading of the active species vanadia is typically between 1 and 5 wt.%, depending on the temperature of operation and the SO2 content in the flue gas. Tungsta adds acid sites, reduces SO2 oxidation, and reduces rutilization of anatase. The typical loading is between 5 and 10 wt.%.
The increased rate of catalyst deactivation experienced in biomass-fired plants is mostly caused by the relatively high alkali- and alkali-earth metal contents in most biomasses [11,17,20–24]. Alkaline metals cause deactivation by neutralizing the catalyst’s acid sites, hence reducing the adsorption of NH3 [13,25–30]. Potassium, in the form of submicron aerosols of mainly KCl and K2SO4 [31–33], is the most important poison due to both its relative abundance and high basicity [24,34]. Equation (1) gives a simplified neutralization reaction with M being any metal.
MCl + V −OH → HCl + V −M (1)
Other modes of deactivation like change in redox properties [35,36] and pore plugging  were reported to be of minor importance.
We have identified four kinds of strategies to deal with the high potassium content in biomasses: (1) potassium removal by adsorption; (2) tail-end placement of the SCR unit; (3) alkali barrier materials on the catalyst surface; and (4) intrinsically potassium resistant catalysts.
2. Strategies Coping with Potassium Rich Fuels
2.1. Potassium Removal by Adsorption
One way of reducing the impact of potassium salts is to minimize the amount taken up by the catalyst bed(s). An obvious strategy is to use an acidic guard bed in front of the catalyst modules. However, due to the high space velocities (5000–10,000 h−1) in SCR units and the high KCl content of about 0.2−1 g Nm−3 of the flue gas [37,38], such a guard bed would probably be saturated too rapidly and require substantial space. Assuming a KCl concentration of 0.2 g Nm−3 in the flue gas, a “guard bed space velocity” of 20,000 h−1, and a monolith density of 300 kg m−3, 1 h of exposure translates into about 180 µmol K per gram. Even highly acidic substances like H-type zeolites with low Si/Al ratios only possess around 5000 µmol of acid sites per gram . To the best of our knowledge, no guard beds have been implemented so far.
Wang et al.  have published a critical review on additives mitigating ash related problems. They have grouped the additives by the following four capture mechanisms: (1) chemical absorption and reaction; (2) physical absorption; (3) dilution and inert elements enrichment and (4) restraining and powdering effects. The first mentioned mechanism was singled out to be the most effective and is based on converting troublesome ash elements into high temperature stable compounds. Additives causing chemical binding can be based on alumino silicates such as, e.g., kaolin, coal fly ash, cat litter, clay minerals, and detergent zeolites. Alumino silicates bind potassium according to the simplified Equation (2).
Al2O3·xSiO2 + 2KCl + H2O→ K2O·Al2O3·SiO2 + 2HCl(g) (2)
Addition of fly ash obtained from coal-fired plants is an industrially used strategy  to bind potassium. Coal fly-ash contains high levels of alumino silicates, which can bind potassium [14,40,41]. Coal fly-ash has the advantage of being abundant and low-cost. Diarmaid et al.  have very recently studied the efficacy of coal-fly ash in reducing the release of potassium from various biomass (white wood pellets, straw, and olive cake) pellets suspended in a methane flame. Additive loadings of 5, 15, and 25 wt.% were used. Olive cake requires larger amounts of alumino silicates to minimize potassium release, probably because it contains more potassium than the other two biomasses. In the presence of additive, up to 100% of K is retained, and in the wood and olive cake ash up to 80% is retained,
Catalysts 2018, 8, 135 3 of 11
demonstrating the effectiveness of alumino silicates even when burning pure biomasses with high potassium contents.
Firing coal with up to 10% [42,43] or even 20%  of biomass has also been reported to result in acceptable catalyst stability, probably because the resulting coal fly ash adsorbs released potassium compounds.
Sulfates of, e.g., ammonia, iron, aluminum, and phosphates of ammonia and calcium, as well as phosphoric acid, have also been listed by Wang et al. A possible issue with using sulfates is an increased formation of SO3. Injection of phosphorous-based “K-getter” compounds leads to the formation of, e.g., K3PO4 and K4P2O7. Dahlin et al.  performed a multivariate analysis of six catalyst poisons (Na, K, Mg, P, S, and Zn) by impregnating monolithic VWT catalysts with corresponding metal precursor solutions. The obtained model showed that P dampens the deactivating effect of K and was explained by the formation of phosphates, preventing the interaction of potassium with vanadia. The effect of K3PO4 on the stability of a vanadia-based catalyst was investigated by Castellino et al.  by exposing full length monoliths to a flue gas containing between 100 mg of K3PO4 per Nm3. 720 h of exposure caused almost 40% deactivation, which was mainly ascribed to potassium neutralizing the catalyst’s acid sites and thereby resembling the deactivation by KCl. The authors concluded that binding K by P is not advantageous to the SCR unit.
2.2. Tail-End Placement of the SCR Unit
Wieck-Hansen et al.  studied the catalyst stability using a slip stream from a 150 MW coal-straw (80%/20%) fired power plant. The catalyst was exposed to the flue gas at 350 C without prior de-dusting, simulating high-dust placement, and at 280 C downstream of a baghouse filter, which reduced the particulate concentration from 100 to a few mg Nm−3, simulating low-dust placement of the SCR unit. 2860 h of high-dust exposure caused about 35% activity loss, while 2350 h of low-dust exposure only caused 15% activity loss. The difference in stability can probably be explained by the removal of, e.g., KCl particles by the dust-filter. Tail-end placement would probably lead to an even higher stability because of the desulphurization unit further reducing the potassium content in the flue gas. Tail-end operation at the biomass co-fired Amager plant in Denmark indeed showed promising results between 2010 and 2012 . Laboratory studies by Putluru et al.  have furthermore shown that heteropoly acid (instead of WO3)-promoted catalysts with a high (3 and 5 wt.%) vanadia loading can retain more than 90% of their activity at 225 C when poisoned with 100 µmol K g−1
catalyst. A corresponding WO3 promoted catalyst lost almost 50% of its activity. At 400 C, the loss was reported to be around 70% . Generally, potassium poisoning has a stronger relative effect at high temperatures [23,48], which is reflected by a lower apparent activation energy upon potassium poisoning , which is consistent with acid neutralization being the main mode of deactivation.
Kristensen et al.  reported excellent potassium tolerance and activity of sol-gel prepared 20 wt.% V2O5/TiO2 at temperatures below 250 C. The potassium loading introduced by KNO3
impregnation was 280 µmol K g−1 catalyst. A commercial reference catalyst got completely deactivated.
The major drawback with tail-end placement is that wet and dry SO2 scrubbers typically reduce the flue gas temperature to about 50 and 150 C, respectively. The VWT catalyst is not active enough at these temperatures, making costly reheating to 180–280 C necessary. Over the last 10 to 15 years, a high number of reports on low-temperature SCR catalysts have appeared . The aim of these studies is to make re-heating redundant. However, most of the reported catalysts are based on manganese, making them extremely sulfur and water sensitive. In 2014, we summarized literature findings on the effects of SO2 and H2O and could not find any convincing reports on sulfur and water-resistant manganese-based catalysts . Here we only give some examples of reports on catalysts being severely affected by SO2 and H2O. Casapu et al.  studied MnCeOx and reported a 79% activity reduction at 150 C by adding 5 vol.% of water to the simulated flue gas. Flue gases typically contain at least 5 vol.% of water. Exposing the same catalyst to 50 ppm of SO2 for 30 min at 250 C reduced the NO conversion from about 70 to 25%. Our group has experienced rapid and severe deactivation
Catalysts 2018, 8, 135 4 of 11
of MnFe/TiO2 and MnFeCe/TiO2 at 150 C by SO2 levels as low as 5 ppm [51,53]. The modes of deactivation were formation of (NH4)2Mn2(SO4)3 and ammonium sulfates. Regeneration by heating to 400 C was only effective with prior washing with base. 20 vol.% of water in the flue gas reduced the NO conversion over a MnFe/TiO2 from over 90% to 30.6%. Doping with ceria did not improve the water tolerance. In 2018, Gao et al.  reviewed the sulfur and water tolerance of Mn-based catalysts at low temperature and concluded, among other things, that more long term studies are needed to validate the viability of this kind of catalyst under realistic conditions.
2.3. Coating Monoliths with Basic Substances
In order to reach the catalyst’s acid sites, potassium, typically originating from submicron aerosols of KCl and K2SO4, first needs to be deposited on the external catalyst (monolith) surface . From there, potassium needs to separate from its counter-ion and diffuse into the catalyst pores, most likely through a surface transport mechanisms involving acid sites [31,55]. In other words, potassium mobility becomes a determining factor in the poisoning mechanism of monolithic samples. A pilot plant study performed by Jensen et al.  investigated the potassium uptake and the resulting deactivation of plate type samples with various WO3 (0, 7 wt.%) and V2O5 (1, 3, 6 wt.%) contents. According to ammonia chemisorptions measurements, both tungsta and vanadia add acid sites to the fresh samples, thereby favoring the potassium uptake. This, in turn, leads to an increased rate of deactivation, e.g., 600 h of KCl aerosol (0.12 µm) at 350 C leads to 76, 81, 89, and 98% relative deactivation for 1%V2O5–0% WO3, 3%V2O5–0% WO3, 1%V2O5–7% WO3, and 3%V2O5–7% WO3, respectively. Based on these results, it is highly questionable if the commonly used strategy of simply increasing the number of surface acid sites is realistic under real life conditions. Despite the just quoted deactivation data, tungsta-free catalysts are not an option for biomass fired plants, because they start from a significantly lower base activity and probably suffer from rutilization over time.
Since the potassium uptake relies on acid sites on the outer monolith surface, it can be reduced by coating this surface with a basic material, thus reducing the relative rate of deactivation [23,56,57]. MgO and Sepiolite (Mg4Si6O15(OH)2·6H2O) have been reported as effective barrier materials. These substances are, on the one hand, basic enough to hinder potassium from penetrating the catalyst wall, and, on the other hand, they do not cause deactivation on their own. Olsen et al.  coated a plate type catalyst with composition of 3 wt.% V2O5–7 wt.% WO3/TiO2 with 8.06 wt.% MgO resulting in a roughly 200µm thick layer and performed a pilot plant exposure campaign with KCl aerosols for several hundred hours at 350 C. The coating layer reduced the rate of deactivation from 0.91% to 0.24% per day. These percentages refer to the initial activity of the uncoated sample. However, the decreased rate of deactivation comes at the cost of an initial activity reduction of about 42%. This activity reduction was ascribed to increased gas phase diffusion limitations introduced by the MgO layer, slight poisoning by MgO on the outer layer of the catalyst, or a combination thereof. SEM-EDS measurements confirmed that the outer MgO layer very effectively prevented potassium from diffusing into the catalyst and that magnesium did not diffuse into the catalyst. Kristensen  very successfully used sepiolite as a binder material for making plate type catalysts from 20 wt.% V2O5/TiO2 powder, reinforced silica sheets, and 20 wt.% sepiolite as binder. The resulting catalyst was exposed to a KCl aerosol for 632 h at 380 C and thereafter crushed to a powder for lab scale activity measurements. A commercial of 3 wt.% V2O5–7 wt.% WO3/TiO2 plate type catalyst was used as reference. When tested at 400 C after KCl exposure, the 20 wt.% V2O5/TiO2-Sepiolite composite retained 68% of its activity, translating into a first order rate constant of about 1650 cm3·g−1·s−1. The activity loss of the reference catalyst was 84%, and the resulting first order rate constant was reported to be only about 200 cm3·g−1·s−1. These activity losses were compared with data from a corresponding incipient wetness (KNO3) poisoning study. The losses experienced by the 20 wt.% V2O5/TiO2-Sepiolite composite and the reference translate into impregnated K loadings of 75 and 172 µmol K g−1
catalyst, strongly suggesting that sepiolite acts as a barrier material. This was confirmed by SEM-EDS measurements, showing that potassium mainly accumulated on the outer surface of the plate.
Catalysts 2018, 8, 135 5 of 11
2.4. Intrinsically Potassium Resistant Catalysts
In this review “intrinsically potassium resistant” refers to catalysts that retain a high share of their activity, even when potassium is taken up from the flue gas and diffuses into the catalysts pore system. To the best of our knowledge, there is up to now no review on potassium tolerant catalysts.
The majority of studies mimic potassium poisoning by impregnation with potassium salts like e.g., KNO3, K2CO3, and KCl followed by calcination. The resulting K-loaded catalysts are typically tested in powder form in lab scale reactors. Studies performed by different laboratories are often difficult to compare due to vastly different experimental conditions and benchmark catalysts. For example, using different potassium loadings and activity testing in different temperature regimes might lead to different conclusions. Benchmarking against catalyst of different potassium tolerance might also lead to different conclusions. Because of these shortcomings in comparability, we start this section with results from our laboratory, which tested a high number of alternative catalysts using identical or very similar experimental conditions.
Figures 1 and 2 present the potassium tolerance for an assortment of catalyst with various active metals (Fe, Cu, and V) and support materials (TiO2, tungsto phosphoric acid (TPA) promoted TiO2, mordernite (MOR), and sulfated ZrO2). The retained activity clearly depends on the number of acid sites of the fresh catalysts, which in turn is very much a function of the support material.
Figure 1. Retained activity at 400 C upon impregnation with 100 µmol K g−1 catalyst. (130 µmol K g−1
catalyst for V2O5/sulfated-ZrO2). Reproduced from .
In this study, the highest alkali tolerance was obtained with MOR (Si/Al = 10)-based catalysts. Putluru et al.  optimized the Cu loading and tested the effect of 0, 250, and 500 µmol K/gcatalyst. 4 wt.% Cu/MOR retains about 60% of its initial activity after poisoning with 500 µmol K g−1
catalyst , while only half that potassium loading causes more than 80% deactivation on a reference catalyst containing 3 wt.% vanadia and 7 wt.% tungsta. Cu/BEA (Si/Al = 25) and Cu/ZSM5 (Si/Al = 15) exhibit only slightly lower potassium tolerance than Cu/MOR does. Cu/Zeolite catalysts are not only very potassium resistant but also very active at 400 C with first order rate constants of up to 1800 cm3g−1s−1, while this value is only about 1000 cm3g−1s−1 for the VWT reference catalyst . Since the high…